#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/49/4114918.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4114918
loop_
_publ_author_name
'Xiqu Wang'
'Lumei Liu'
'Allan J. Jacobson'
_publ_contact_author_address
;
Department of Chemistry    
University of Houston,
Houston, TX 77204-5003
;
_publ_contact_author_email       ' ajjcob@uh.edu '
_publ_contact_author_fax         ' 713 743 2787 '
_publ_contact_author_name
;
Prof. Allan J. Jacobson
;
_publ_contact_author_phone       ' 713 743 2785 '
_publ_section_title
;
 Open-Framework and Microporous Vanadium Silicates
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7812
_journal_page_last               7820
_journal_paper_doi               10.1021/ja020354l
_journal_volume                  124
_journal_year                    2002
_chemical_formula_sum            'Cs2 H2 O12 Si4 V'
_chemical_formula_weight         623.14
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           55
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_atom_sites_solution_hydrogens   IGNORED
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.689(3)
_cell_length_b                   14.915(3)
_cell_length_c                   6.9835(14)
_cell_measurement_temperature    293(2)
_cell_volume                     1321.7(5)
_computing_cell_refinement       SAINT
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    SHELXTL
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.947
_diffrn_measured_fraction_theta_max 0.947
_diffrn_measurement_device_type  'SIEMENS SMART/CCD'
_diffrn_measurement_method       'NARROW FRAME, 0.3w'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0782
_diffrn_reflns_av_sigmaI/netI    0.0550
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            7916
_diffrn_reflns_theta_full        28.41
_diffrn_reflns_theta_max         28.41
_diffrn_reflns_theta_min         2.11
_exptl_absorpt_coefficient_mu    6.595
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.3680
_exptl_absorpt_correction_type   'multi-scan (SADABS)'
_exptl_crystal_colour            BLUE-GREEN
_exptl_crystal_density_diffrn    3.132
_exptl_crystal_description       PRISM
_exptl_crystal_F_000             1148
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.10
_refine_diff_density_max         1.364
_refine_diff_density_min         -1.541
_refine_diff_density_rms         0.271
_refine_ls_extinction_coef       0.0005(1)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.261
_refine_ls_hydrogen_treatment    NA
_refine_ls_matrix_type           full
_refine_ls_number_parameters     154
_refine_ls_number_reflns         1706
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.261
_refine_ls_R_factor_all          0.1314
_refine_ls_R_factor_gt           0.1131
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0001P)²+68.9692P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2378
_refine_ls_wR_factor_ref         0.2443
_reflns_number_gt                1393
_reflns_number_total             1706
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja020354l_09.cif
_cod_data_source_block           VSH-12Cs
_cod_original_formula_sum        'H2 Cs2 O12 Si4 V'
_cod_database_code               4114918
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x-1/2, -y-1/2, z'
'-x-1/2, y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cs1 Cs 0.1549(7) 0.0769(5) 0.0000 0.059(3) Uani 0.64(4) 2 d SP
Cs2 Cs 0.5765(6) 0.1522(7) 0.5000 0.047(3) Uani 0.48(2) 2 d SP
Cs3 Cs 0.174(3) 0.0841(14) 0.092(8) 0.151(17) Uani 0.20(2) 1 d P
Cs4 Cs 0.327(2) 0.034(2) 0.5000 0.090(9) Uani 0.187(17) 2 d SP
Cs5 Cs 0.3579(8) 0.1008(15) 0.5000 0.048(4) Uani 0.212(18) 2 d SP
Cs6 Cs 0.608(2) 0.205(3) 0.5000 0.018(9) Uiso 0.048(9) 2 d SP
Cs7 Cs 0.627(2) 0.254(2) 0.5000 0.021(9) Uiso 0.046(7) 2 d SP
V1 V 0.5000 0.0000 0.0000 0.0227(11) Uani 1 4 d S
V2 V 0.0280(7) 0.0343(6) 0.5000 0.040(2) Uani 0.50 2 d SP
Si1 Si 0.6925(3) 0.1375(3) 0.0000 0.0175(11) Uani 1 2 d S
Si2 Si 0.4788(3) 0.2125(3) 0.0000 0.0149(10) Uani 1 2 d S
Si3 Si 0.8747(3) 0.1587(4) 0.2895(5) 0.0402(13) Uani 1 1 d .
O1 O 0.6052(11) 0.2141(9) 0.0000 0.072(8) Uani 1 2 d S
O2 O 0.9332(11) 0.0655(9) 0.3020(15) 0.057(3) Uani 1 1 d .
O3 O 0.7642(10) 0.1512(14) 0.1796(18) 0.091(6) Uani 1 1 d .
O4 O 0.848(2) 0.1989(16) 0.5000 0.081(8) Uani 1 2 d S
O5 O 0.4419(15) 0.2686(13) 0.1768(19) 0.107(8) Uani 1 1 d .
O6 O 0.4408(12) 0.1162(10) 0.0000 0.144(17) Uani 1 2 d S
O7 O 0.6391(12) 0.0461(9) 0.0000 0.132(16) Uani 1 2 d S
O8 O 0.5000 0.0000 0.241(5) 0.062(11) Uani 0.50 2 d SP
O9 O 0.133(4) 0.106(2) 0.5000 0.071(13) Uani 0.50 2 d SP
OW1 O 0.654(4) 0.296(4) 0.5000 0.021(12) Uiso 0.236(17) 2 d SP
OW2 O 0.373(4) 0.063(5) 0.5000 0.021(8) Uiso 0.47(12) 2 d SP
OW3 O 0.540(6) 0.127(3) 0.5000 0.021(8) Uiso 0.39(12) 2 d SP
OW4 O 0.051(12) 0.111(10) 0.0000 0.021(8) Uiso 0.08(3) 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Cs3 Cs1 Cs3 136(5) . 6
Cs3 Cs1 OW4 105(3) . .
Cs3 Cs1 OW4 105(3) 6 .
Cs3 Cs1 O1 85.2(17) . 7_565
Cs3 Cs1 O1 85.2(17) 6 7_565
OW4 Cs1 O1 58(6) . 7_565
Cs3 Cs1 O7 79(2) . 5_655
Cs3 Cs1 O7 79(2) 6 5_655
OW4 Cs1 O7 166(6) . 5_655
O1 Cs1 O7 136.5(5) 7_565 5_655
Cs3 Cs1 O2 147(2) . 5_655
Cs3 Cs1 O2 67(2) 6 5_655
OW4 Cs1 O2 85(5) . 5_655
O1 Cs1 O2 125.6(3) 7_565 5_655
O7 Cs1 O2 84.5(3) 5_655 5_655
Cs3 Cs1 O2 67(2) . 2_655
Cs3 Cs1 O2 147(2) 6 2_655
OW4 Cs1 O2 85(5) . 2_655
O1 Cs1 O2 125.6(3) 7_565 2_655
O7 Cs1 O2 84.5(3) 5_655 2_655
O2 Cs1 O2 82.6(5) 5_655 2_655
Cs3 Cs1 O2 147(2) . 6_455
Cs3 Cs1 O2 74(2) 6 6_455
OW4 Cs1 O2 43(3) . 6_455
O1 Cs1 O2 83.6(3) 7_565 6_455
O7 Cs1 O2 128.8(3) 5_655 6_455
O2 Cs1 O2 45.0(5) 5_655 6_455
O2 Cs1 O2 94.8(4) 2_655 6_455
Cs3 Cs1 O2 74(2) . 1_455
Cs3 Cs1 O2 147(2) 6 1_455
OW4 Cs1 O2 43(3) . 1_455
O1 Cs1 O2 83.6(3) 7_565 1_455
O7 Cs1 O2 128.8(3) 5_655 1_455
O2 Cs1 O2 94.8(4) 5_655 1_455
O2 Cs1 O2 45.0(5) 2_655 1_455
O2 Cs1 O2 73.6(4) 6_455 1_455
Cs3 Cs1 O9 25(2) . .
Cs3 Cs1 O9 158(3) 6 .
OW4 Cs1 O9 83.2(10) . .
O1 Cs1 O9 82.2(6) 7_565 .
O7 Cs1 O9 97.8(8) 5_655 .
O2 Cs1 O9 134.9(7) 5_655 .
O2 Cs1 O9 53.1(6) 2_655 .
O2 Cs1 O9 122.3(9) 6_455 .
O2 Cs1 O9 49.4(8) 1_455 .
Cs3 Cs1 O9 158(3) . 1_554
Cs3 Cs1 O9 25(2) 6 1_554
OW4 Cs1 O9 83.2(10) . 1_554
O1 Cs1 O9 82.2(6) 7_565 1_554
O7 Cs1 O9 97.8(8) 5_655 1_554
O2 Cs1 O9 53.1(6) 5_655 1_554
O2 Cs1 O9 134.9(7) 2_655 1_554
O2 Cs1 O9 49.4(8) 6_455 1_554
O2 Cs1 O9 122.3(9) 1_455 1_554
O9 Cs1 O9 163.3(15) . 1_554
Cs3 Cs1 O6 69(2) . .
Cs3 Cs1 O6 69(2) 6 .
OW4 Cs1 O6 150(6) . .
O1 Cs1 O6 92.3(4) 7_565 .
O7 Cs1 O6 44.2(4) 5_655 .
O2 Cs1 O6 116.8(3) 5_655 .
O2 Cs1 O6 116.8(3) 2_655 .
O2 Cs1 O6 142.8(2) 6_455 .
O2 Cs1 O6 142.8(2) 1_455 .
O9 Cs1 O6 93.4(8) . .
O9 Cs1 O6 93.4(8) 1_554 .
OW3 Cs2 Cs6 156(6) . .
OW3 Cs2 Cs7 152(6) . .
Cs6 Cs2 Cs7 4.1(19) . .
OW3 Cs2 OW1 153(6) . .
Cs6 Cs2 OW1 2(2) . .
Cs7 Cs2 OW1 1.7(16) . .
OW3 Cs2 Cs5 23(6) . .
Cs6 Cs2 Cs5 132.3(17) . .
Cs7 Cs2 Cs5 128.3(10) . .
OW1 Cs2 Cs5 129.9(14) . .
OW3 Cs2 OW2 11(6) . .
Cs6 Cs2 OW2 144(2) . .
Cs7 Cs2 OW2 140.1(17) . .
OW1 Cs2 OW2 142(2) . .
Cs5 Cs2 OW2 11.9(11) . .
OW3 Cs2 Cs4 75(6) . 5_656
Cs6 Cs2 Cs4 129.3(17) . 5_656
Cs7 Cs2 Cs4 133.4(12) . 5_656
OW1 Cs2 Cs4 131.7(15) . 5_656
Cs5 Cs2 Cs4 98.3(9) . 5_656
OW2 Cs2 Cs4 86.5(16) . 5_656
OW3 Cs2 O8 45(3) . .
Cs6 Cs2 O8 143.6(5) . .
Cs7 Cs2 O8 143.8(5) . .
OW1 Cs2 O8 143.8(5) . .
Cs5 Cs2 O8 59.8(5) . .
OW2 Cs2 O8 51.5(11) . .
Cs4 Cs2 O8 56.6(6) 5_656 .
OW3 Cs2 O8 45(3) . 5_656
Cs6 Cs2 O8 143.6(5) . 5_656
Cs7 Cs2 O8 143.8(5) . 5_656
OW1 Cs2 O8 143.8(5) . 5_656
Cs5 Cs2 O8 59.8(5) . 5_656
OW2 Cs2 O8 51.5(11) . 5_656
Cs4 Cs2 O8 56.6(6) 5_656 5_656
O8 Cs2 O8 72.4(10) . 5_656
OW3 Cs2 O3 124(3) . 6_556
Cs6 Cs2 O3 71.0(12) . 6_556
Cs7 Cs2 O3 73.9(8) . 6_556
OW1 Cs2 O3 72.7(10) . 6_556
Cs5 Cs2 O3 134.5(4) . 6_556
OW2 Cs2 O3 130.2(8) . 6_556
Cs4 Cs2 O3 72.6(6) 5_656 6_556
O8 Cs2 O3 129.2(5) . 6_556
O8 Cs2 O3 79.8(5) 5_656 6_556
OW3 Cs2 O3 124(3) . .
Cs6 Cs2 O3 71.0(12) . .
Cs7 Cs2 O3 73.9(8) . .
OW1 Cs2 O3 72.7(10) . .
Cs5 Cs2 O3 134.5(4) . .
OW2 Cs2 O3 130.2(8) . .
Cs4 Cs2 O3 72.6(6) 5_656 .
O8 Cs2 O3 79.8(5) . .
O8 Cs2 O3 129.2(5) 5_656 .
O3 Cs2 O3 86.4(5) 6_556 .
OW3 Cs2 OW2 63(6) . 5_656
Cs6 Cs2 OW2 141.7(18) . 5_656
Cs7 Cs2 OW2 145.8(14) . 5_656
OW1 Cs2 OW2 144.1(16) . 5_656
Cs5 Cs2 OW2 85.9(12) . 5_656
OW2 Cs2 OW2 74.1(19) . 5_656
Cs4 Cs2 OW2 12.4(7) 5_656 5_656
O8 Cs2 OW2 48.3(7) . 5_656
O8 Cs2 OW2 48.3(7) 5_656 5_656
O3 Cs2 OW2 81.4(7) 6_556 5_656
O3 Cs2 OW2 81.4(7) . 5_656
Cs1 Cs3 Cs3 22(2) . 6
Cs1 Cs3 OW4 52(4) . .
Cs3 Cs3 OW4 68(2) 6 .
Cs1 Cs3 O9 149(3) . .
Cs3 Cs3 O9 167.9(12) 6 .
OW4 Cs3 O9 100(2) . .
Cs1 Cs3 O2 100(3) . 2_655
Cs3 Cs3 O2 119.3(12) 6 2_655
OW4 Cs3 O2 87(5) . 2_655
O9 Cs3 O2 61.5(9) . 2_655
Cs1 Cs3 O7 88.6(16) . 5_655
Cs3 Cs3 O7 78.1(10) 6 5_655
OW4 Cs3 O7 138(4) . 5_655
O9 Cs3 O7 113.9(19) . 5_655
O2 Cs3 O7 89.0(5) 2_655 5_655
Cs1 Cs3 O1 82(2) . 7_565
Cs3 Cs3 O1 78.4(9) 6 7_565
OW4 Cs3 O1 58(5) . 7_565
O9 Cs3 O1 92.5(11) . 7_565
O2 Cs3 O1 132.6(7) 2_655 7_565
O7 Cs3 O1 138.4(6) 5_655 7_565
Cs1 Cs3 OW1 147(3) . 7_565
Cs3 Cs3 OW1 147.7(10) 6 7_565
OW4 Cs3 OW1 97(3) . 7_565
O9 Cs3 OW1 26.0(12) . 7_565
O2 Cs3 OW1 86.9(13) 2_655 7_565
O7 Cs3 OW1 124(2) 5_655 7_565
O1 Cs3 OW1 69.6(11) 7_565 7_565
Cs1 Cs3 O2 94(3) . 1_455
Cs3 Cs3 O2 115.6(11) 6 1_455
OW4 Cs3 O2 51(3) . 1_455
O9 Cs3 O2 55.0(10) . 1_455
O2 Cs3 O2 47.2(5) 2_655 1_455
O7 Cs3 O2 135.9(6) 5_655 1_455
O1 Cs3 O2 85.4(5) 7_565 1_455
OW1 Cs3 O2 67.1(10) 7_565 1_455
Cs1 Cs3 V2 123(3) . .
Cs3 Cs3 V2 145.0(11) 6 .
OW4 Cs3 V2 83(3) . .
O9 Cs3 V2 29.2(8) . .
O2 Cs3 V2 36.7(4) 2_655 .
O7 Cs3 V2 116.0(9) 5_655 .
O1 Cs3 V2 102.8(5) 7_565 .
OW1 Cs3 V2 51.7(10) 7_565 .
O2 Cs3 V2 31.9(3) 1_455 .
Cs1 Cs3 O6 100.7(18) . .
Cs3 Cs3 O6 79.3(10) 6 .
OW4 Cs3 O6 141(4) . .
O9 Cs3 O6 110(2) . .
O2 Cs3 O6 129.3(11) 2_655 .
O7 Cs3 O6 46.4(5) 5_655 .
O1 Cs3 O6 95.6(7) 7_565 .
OW1 Cs3 O6 99.0(18) 7_565 .
O2 Cs3 O6 165(2) 1_455 .
V2 Cs3 O6 134.3(19) . .
Cs1 Cs3 Cs4 154.9(19) . .
Cs3 Cs3 Cs4 143.9(4) 6 .
OW4 Cs3 Cs4 147(2) . .
O9 Cs3 Cs4 48.1(14) . .
O2 Cs3 Cs4 72.4(11) 2_655 .
O7 Cs3 Cs4 67.6(9) 5_655 .
O1 Cs3 Cs4 120.7(17) 7_565 .
OW1 Cs3 Cs4 58.0(15) 7_565 .
O2 Cs3 Cs4 97.4(11) 1_455 .
V2 Cs3 Cs4 65.6(10) . .
O6 Cs3 Cs4 69.0(11) . .
OW2 Cs4 Cs5 32(5) . .
OW2 Cs4 O9 121(6) . .
Cs5 Cs4 O9 88.4(16) . .
OW2 Cs4 O8 59(4) . 5_656
Cs5 Cs4 O8 83.3(16) . 5_656
O9 Cs4 O8 140.2(6) . 5_656
OW2 Cs4 O8 59(4) . .
Cs5 Cs4 O8 83.3(16) . .
O9 Cs4 O8 140.2(6) . .
O8 Cs4 O8 77.4(12) 5_656 .
OW2 Cs4 OW3 91(6) . 5_656
Cs5 Cs4 OW3 123(3) . 5_656
O9 Cs4 OW3 148(2) . 5_656
O8 Cs4 OW3 54.3(10) 5_656 5_656
O8 Cs4 OW3 54.3(10) . 5_656
OW2 Cs4 OW3 9(6) . .
Cs5 Cs4 OW3 41.2(18) . .
O9 Cs4 OW3 129.6(17) . .
O8 Cs4 OW3 53.4(8) 5_656 .
O8 Cs4 OW3 53.4(8) . .
OW3 Cs4 OW3 81.9(17) 5_656 .
OW2 Cs4 Cs2 102(6) . 5_656
Cs5 Cs4 Cs2 134(2) . 5_656
O9 Cs4 Cs2 137.1(16) . 5_656
O8 Cs4 Cs2 62.0(4) 5_656 5_656
O8 Cs4 Cs2 62.0(4) . 5_656
OW3 Cs4 Cs2 11.3(13) 5_656 5_656
OW3 Cs4 Cs2 93.3(11) . 5_656
OW2 Cs4 OW1 95(6) . 7_565
Cs5 Cs4 OW1 62.8(16) . 7_565
O9 Cs4 OW1 25.6(11) . 7_565
O8 Cs4 OW1 129.3(10) 5_656 7_565
O8 Cs4 OW1 129.3(10) . 7_565
OW3 Cs4 OW1 174(2) 5_656 7_565
OW3 Cs4 OW1 104.0(17) . 7_565
Cs2 Cs4 OW1 162.8(17) 5_656 7_565
OW2 Cs4 Cs3 109(3) . .
Cs5 Cs4 Cs3 90.5(10) . .
O9 Cs4 Cs3 53.9(4) . .
O8 Cs4 Cs3 163.9(10) 5_656 .
O8 Cs4 Cs3 87.2(5) . .
OW3 Cs4 Cs3 119.3(9) 5_656 .
OW3 Cs4 Cs3 113.2(10) . .
Cs2 Cs4 Cs3 114.5(8) 5_656 .
OW1 Cs4 Cs3 58.7(6) 7_565 .
OW2 Cs4 Cs3 109(3) . 6_556
Cs5 Cs4 Cs3 90.5(10) . 6_556
O9 Cs4 Cs3 53.9(4) . 6_556
O8 Cs4 Cs3 87.2(5) 5_656 6_556
O8 Cs4 Cs3 163.9(10) . 6_556
OW3 Cs4 Cs3 119.3(9) 5_656 6_556
OW3 Cs4 Cs3 113.2(10) . 6_556
Cs2 Cs4 Cs3 114.5(8) 5_656 6_556
OW1 Cs4 Cs3 58.7(6) 7_565 6_556
Cs3 Cs4 Cs3 107.8(7) . 6_556
OW2 Cs4 Cs2 7(6) . .
Cs5 Cs4 Cs2 39.2(15) . .
O9 Cs4 Cs2 127.7(12) . .
O8 Cs4 Cs2 54.6(7) 5_656 .
O8 Cs4 Cs2 54.6(7) . .
OW3 Cs4 Cs2 83.8(17) 5_656 .
OW3 Cs4 Cs2 1.9(10) . .
Cs2 Cs4 Cs2 95.2(7) 5_656 .
OW1 Cs4 Cs2 102.0(12) 7_565 .
Cs3 Cs4 Cs2 112.3(8) . .
Cs3 Cs4 Cs2 112.3(8) 6_556 .
OW2 Cs5 Cs4 40(5) . .
OW2 Cs5 OW3 81(6) . .
Cs4 Cs5 OW3 121(2) . .
OW2 Cs5 O9 110(5) . .
Cs4 Cs5 O9 69.7(16) . .
OW3 Cs5 O9 168.9(17) . .
OW2 Cs5 Cs2 87(5) . .
Cs4 Cs5 Cs2 127.2(19) . .
OW3 Cs5 Cs2 5.8(12) . .
O9 Cs5 Cs2 163.1(12) . .
OW2 Cs5 O8 48(3) . 5_656
Cs4 Cs5 O8 75.8(14) . 5_656
OW3 Cs5 O8 59.0(9) . 5_656
O9 Cs5 O8 128.4(7) . 5_656
Cs2 Cs5 O8 63.2(3) . 5_656
OW2 Cs5 O8 48(3) . .
Cs4 Cs5 O8 75.8(14) . .
OW3 Cs5 O8 59.0(9) . .
O9 Cs5 O8 128.4(7) . .
Cs2 Cs5 O8 63.2(3) . .
O8 Cs5 O8 75.2(11) 5_656 .
OW2 Cs5 O4 164(5) . 7_565
Cs4 Cs5 O4 155.8(18) . 7_565
OW3 Cs5 O4 82.8(14) . 7_565
O9 Cs5 O4 86.1(10) . 7_565
Cs2 Cs5 O4 76.9(7) . 7_565
O8 Cs5 O4 122.2(6) 5_656 7_565
O8 Cs5 O4 122.2(6) . 7_565
OW2 Cs5 OW1 139(5) . 7_565
Cs4 Cs5 OW1 98.8(18) . 7_565
OW3 Cs5 OW1 139.8(17) . 7_565
O9 Cs5 OW1 29.1(13) . 7_565
Cs2 Cs5 OW1 133.9(13) . 7_565
O8 Cs5 OW1 141.4(5) 5_656 7_565
O8 Cs5 OW1 141.4(5) . 7_565
O4 Cs5 OW1 57.0(12) 7_565 7_565
OW2 Cs5 Cs6 98(5) . .
Cs4 Cs5 Cs6 137.8(19) . .
OW3 Cs5 Cs6 16.4(12) . .
O9 Cs5 Cs6 152.5(12) . .
Cs2 Cs5 Cs6 10.6(6) . .
O8 Cs5 Cs6 71.1(5) 5_656 .
O8 Cs5 Cs6 71.1(5) . .
O4 Cs5 Cs6 66.4(8) 7_565 .
OW1 Cs5 Cs6 123.3(13) 7_565 .
OW2 Cs5 O5 125(3) . 6_556
Cs4 Cs5 O5 140.3(3) . 6_556
OW3 Cs5 O5 65.4(9) . 6_556
O9 Cs5 O5 106.5(8) . 6_556
Cs2 Cs5 O5 61.4(4) . 6_556
O8 Cs5 O5 77.6(4) 5_656 6_556
O8 Cs5 O5 124.4(5) . 6_556
O4 Cs5 O5 46.0(4) 7_565 6_556
OW1 Cs5 O5 84.2(10) 7_565 6_556
Cs6 Cs5 O5 54.4(5) . 6_556
OW2 Cs5 O5 125(3) . .
Cs4 Cs5 O5 140.3(3) . .
OW3 Cs5 O5 65.4(9) . .
O9 Cs5 O5 106.5(8) . .
Cs2 Cs5 O5 61.4(4) . .
O8 Cs5 O5 124.4(5) 5_656 .
O8 Cs5 O5 77.6(4) . .
O4 Cs5 O5 46.0(4) 7_565 .
OW1 Cs5 O5 84.2(10) 7_565 .
Cs6 Cs5 O5 54.4(5) . .
O5 Cs5 O5 79.4(6) 6_556 .
Cs7 Cs6 Cs2 171(4) . .
Cs7 Cs6 OW3 161(4) . .
Cs2 Cs6 OW3 10(3) . .
Cs7 Cs6 OW1 5(3) . .
Cs2 Cs6 OW1 176(3) . .
OW3 Cs6 OW1 166(4) . .
Cs7 Cs6 O9 12(3) . 7_665
Cs2 Cs6 O9 159(2) . 7_665
OW3 Cs6 O9 150(3) . 7_665
OW1 Cs6 O9 17(2) . 7_665
Cs7 Cs6 O4 73(3) . .
Cs2 Cs6 O4 115(2) . .
OW3 Cs6 O4 125(3) . .
OW1 Cs6 O4 69(2) . .
O9 Cs6 O4 85.2(15) 7_665 .
Cs7 Cs6 O3 93(2) . 6_556
Cs2 Cs6 O3 93.4(15) . 6_556
OW3 Cs6 O3 100.2(19) . 6_556
OW1 Cs6 O3 89.2(18) . 6_556
O9 Cs6 O3 100.7(13) 7_665 6_556
O4 Cs6 O3 49.6(5) . 6_556
Cs7 Cs6 O3 93(2) . .
Cs2 Cs6 O3 93.4(15) . .
OW3 Cs6 O3 100.2(19) . .
OW1 Cs6 O3 89.2(18) . .
O9 Cs6 O3 100.7(13) 7_665 .
O4 Cs6 O3 49.6(5) . .
O3 Cs6 O3 92.6(8) 6_556 .
Cs7 Cs6 O5 86(2) . .
Cs2 Cs6 O5 88.2(14) . .
OW3 Cs6 O5 81(2) . .
OW1 Cs6 O5 89.1(18) . .
O9 Cs6 O5 77.2(10) 7_665 .
O4 Cs6 O5 131.3(8) . .
O3 Cs6 O5 177.4(12) 6_556 .
O3 Cs6 O5 89.4(4) . .
Cs7 Cs6 O5 86(2) . 6_556
Cs2 Cs6 O5 88.2(14) . 6_556
OW3 Cs6 O5 81(2) . 6_556
OW1 Cs6 O5 89.1(18) . 6_556
O9 Cs6 O5 77.2(10) 7_665 6_556
O4 Cs6 O5 131.3(8) . 6_556
O3 Cs6 O5 89.4(4) 6_556 6_556
O3 Cs6 O5 177.4(12) . 6_556
O5 Cs6 O5 88.7(8) . 6_556
Cs7 Cs6 O1 88.0(8) . 1_556
Cs2 Cs6 O1 91.8(8) . 1_556
OW3 Cs6 O1 91.5(8) . 1_556
OW1 Cs6 O1 88.1(8) . 1_556
O9 Cs6 O1 87.8(7) 7_665 1_556
O4 Cs6 O1 90.6(5) . 1_556
O3 Cs6 O1 45.1(3) 6_556 1_556
O3 Cs6 O1 137.6(8) . 1_556
O5 Cs6 O1 132.9(8) . 1_556
O5 Cs6 O1 44.3(4) 6_556 1_556
Cs7 Cs6 O1 88.0(8) . .
Cs2 Cs6 O1 91.8(8) . .
OW3 Cs6 O1 91.5(8) . .
OW1 Cs6 O1 88.1(8) . .
O9 Cs6 O1 87.8(7) 7_665 .
O4 Cs6 O1 90.6(5) . .
O3 Cs6 O1 137.6(8) 6_556 .
O3 Cs6 O1 45.1(3) . .
O5 Cs6 O1 44.3(4) . .
O5 Cs6 O1 132.9(8) 6_556 .
O1 Cs6 O1 175.3(13) 1_556 .
OW1 Cs7 Cs6 170(6) . .
OW1 Cs7 Cs2 174(5) . .
Cs6 Cs7 Cs2 5(2) . .
OW1 Cs7 O9 26(5) . 7_665
Cs6 Cs7 O9 164(4) . 7_665
Cs2 Cs7 O9 159(2) . 7_665
OW1 Cs7 OW3 178(6) . .
Cs6 Cs7 OW3 12(3) . .
Cs2 Cs7 OW3 7.5(18) . .
O9 Cs7 OW3 152(3) 7_665 .
OW1 Cs7 O4 78(5) . .
Cs6 Cs7 O4 92(3) . .
Cs2 Cs7 O4 96.6(13) . .
O9 Cs7 O4 104.1(19) 7_665 .
OW3 Cs7 O4 104(2) . .
OW1 Cs7 O3 99(4) . 6_556
Cs6 Cs7 O3 74(2) . 6_556
Cs2 Cs7 O3 76.8(9) . 6_556
O9 Cs7 O3 117.0(13) 7_665 6_556
OW3 Cs7 O3 82.2(15) . 6_556
O4 Cs7 O3 49.3(5) . 6_556
OW1 Cs7 O3 99(4) . .
Cs6 Cs7 O3 74(2) . .
Cs2 Cs7 O3 76.8(9) . .
O9 Cs7 O3 117.0(13) 7_665 .
OW3 Cs7 O3 82.2(15) . .
O4 Cs7 O3 49.3(5) . .
O3 Cs7 O3 87.9(8) 6_556 .
OW1 Cs7 O5 106(4) . .
Cs6 Cs7 O5 81(2) . .
Cs2 Cs7 O5 77.5(9) . .
O9 Cs7 O5 87.6(13) 7_665 .
OW3 Cs7 O5 72.3(15) . .
O4 Cs7 O5 135.2(5) . .
O3 Cs7 O5 154.4(13) 6_556 .
O3 Cs7 O5 86.6(4) . .
OW1 Cs7 O5 106(4) . 6_556
Cs6 Cs7 O5 81(2) . 6_556
Cs2 Cs7 O5 77.5(9) . 6_556
O9 Cs7 O5 87.6(13) 7_665 6_556
OW3 Cs7 O5 72.3(15) . 6_556
O4 Cs7 O5 135.2(5) . 6_556
O3 Cs7 O5 86.6(4) 6_556 6_556
O3 Cs7 O5 154.4(13) . 6_556
O5 Cs7 O5 87.6(9) . 6_556
OW1 Cs7 V2 50(5) . 7_665
Cs6 Cs7 V2 140(3) . 7_665
Cs2 Cs7 V2 135.6(12) . 7_665
O9 Cs7 V2 23.7(14) 7_665 7_665
OW3 Cs7 V2 128(2) . 7_665
O4 Cs7 V2 127.8(12) . 7_665
O3 Cs7 V2 129.8(7) 6_556 7_665
O3 Cs7 V2 129.8(7) . 7_665
O5 Cs7 V2 70.9(6) . 7_665
O5 Cs7 V2 70.9(6) 6_556 7_665
OW1 Cs7 O1 100.5(6) . .
Cs6 Cs7 O1 79.5(6) . .
Cs2 Cs7 O1 79.4(6) . .
O9 Cs7 O1 99.7(6) 7_665 .
OW3 Cs7 O1 79.5(6) . .
O4 Cs7 O1 91.6(5) . .
O3 Cs7 O1 130.2(9) 6_556 .
O3 Cs7 O1 44.0(3) . .
O5 Cs7 O1 43.6(4) . .
O5 Cs7 O1 129.5(9) 6_556 .
V2 Cs7 O1 97.3(5) 7_665 .
O8 V1 O8 180.000(1) . 5_655
O8 V1 O6 90.0 . 5_655
O8 V1 O6 90.0 5_655 5_655
O8 V1 O6 90.0 . .
O8 V1 O6 90.0 5_655 .
O6 V1 O6 180.0(10) 5_655 .
O8 V1 O7 90.0 . 5_655
O8 V1 O7 90.0 5_655 5_655
O6 V1 O7 92.1(6) 5_655 5_655
O6 V1 O7 87.9(6) . 5_655
O8 V1 O7 90.0 . .
O8 V1 O7 90.0 5_655 .
O6 V1 O7 87.9(6) 5_655 .
O6 V1 O7 92.1(6) . .
O7 V1 O7 180.0(9) 5_655 .
O8 V1 Cs4 147.1(3) . 1_554
O8 V1 Cs4 32.9(3) 5_655 1_554
O6 V1 Cs4 108.9(4) 5_655 1_554
O6 V1 Cs4 71.1(4) . 1_554
O7 V1 Cs4 63.4(5) 5_655 1_554
O7 V1 Cs4 116.6(5) . 1_554
O8 V1 Cs4 32.9(3) . 5_656
O8 V1 Cs4 147.1(3) 5_655 5_656
O6 V1 Cs4 71.1(4) 5_655 5_656
O6 V1 Cs4 108.9(4) . 5_656
O7 V1 Cs4 116.6(5) 5_655 5_656
O7 V1 Cs4 63.4(5) . 5_656
Cs4 V1 Cs4 180.0(8) 1_554 5_656
O8 V1 Cs4 32.9(3) . .
O8 V1 Cs4 147.1(3) 5_655 .
O6 V1 Cs4 108.9(4) 5_655 .
O6 V1 Cs4 71.1(4) . .
O7 V1 Cs4 63.4(5) 5_655 .
O7 V1 Cs4 116.6(5) . .
Cs4 V1 Cs4 114.2(6) 1_554 .
Cs4 V1 Cs4 65.8(6) 5_656 .
O8 V1 Cs4 147.1(3) . 5_655
O8 V1 Cs4 32.9(3) 5_655 5_655
O6 V1 Cs4 71.1(4) 5_655 5_655
O6 V1 Cs4 108.9(4) . 5_655
O7 V1 Cs4 116.6(5) 5_655 5_655
O7 V1 Cs4 63.4(5) . 5_655
Cs4 V1 Cs4 65.8(6) 1_554 5_655
Cs4 V1 Cs4 114.2(6) 5_656 5_655
Cs4 V1 Cs4 180.000(1) . 5_655
O8 V1 Cs5 146.1(2) . 1_554
O8 V1 Cs5 33.9(2) 5_655 1_554
O6 V1 Cs5 119.9(3) 5_655 1_554
O6 V1 Cs5 60.1(3) . 1_554
O7 V1 Cs5 74.3(3) 5_655 1_554
O7 V1 Cs5 105.7(3) . 1_554
Cs4 V1 Cs5 14.6(5) 1_554 1_554
Cs4 V1 Cs5 165.4(5) 5_656 1_554
Cs4 V1 Cs5 115.2(2) . 1_554
Cs4 V1 Cs5 64.8(2) 5_655 1_554
O8 V1 Cs5 33.9(2) . .
O8 V1 Cs5 146.1(2) 5_655 .
O6 V1 Cs5 119.9(3) 5_655 .
O6 V1 Cs5 60.1(3) . .
O7 V1 Cs5 74.3(3) 5_655 .
O7 V1 Cs5 105.7(3) . .
Cs4 V1 Cs5 115.2(2) 1_554 .
Cs4 V1 Cs5 64.8(2) 5_656 .
Cs4 V1 Cs5 14.6(5) . .
Cs4 V1 Cs5 165.4(5) 5_655 .
Cs5 V1 Cs5 112.2(4) 1_554 .
V2 V2 O9 164(2) 5_556 .
V2 V2 O2 80.8(7) 5_556 1_455
O9 V2 O2 110.0(11) . 1_455
V2 V2 O2 80.8(7) 5_556 6_456
O9 V2 O2 110.0(11) . 6_456
O2 V2 O2 94.0(9) 1_455 6_456
V2 V2 O2 63.2(6) 5_556 2_655
O9 V2 O2 105.2(13) . 2_655
O2 V2 O2 80.9(7) 1_455 2_655
O2 V2 O2 144.0(5) 6_456 2_655
V2 V2 O2 63.2(6) 5_556 5_656
O9 V2 O2 105.2(13) . 5_656
O2 V2 O2 144.0(5) 1_455 5_656
O2 V2 O2 80.9(7) 6_456 5_656
O2 V2 O2 82.8(7) 2_655 5_656
V2 V2 Cs7 166.8(11) 5_556 7_565
O9 V2 Cs7 29.6(17) . 7_565
O2 V2 Cs7 90.3(6) 1_455 7_565
O2 V2 Cs7 90.3(6) 6_456 7_565
O2 V2 Cs7 125.1(5) 2_655 7_565
O2 V2 Cs7 125.1(5) 5_656 7_565
V2 V2 Cs3 118.6(9) 5_556 6_556
O9 V2 Cs3 56.7(10) . 6_556
O2 V2 Cs3 152.2(6) 1_455 6_556
O2 V2 Cs3 71.7(10) 6_456 6_556
O2 V2 Cs3 124.7(7) 2_655 6_556
O2 V2 Cs3 59.0(7) 5_656 6_556
Cs7 V2 Cs3 66.7(7) 7_565 6_556
V2 V2 Cs3 118.6(9) 5_556 .
O9 V2 Cs3 56.7(10) . .
O2 V2 Cs3 71.7(10) 1_455 .
O2 V2 Cs3 152.2(6) 6_456 .
O2 V2 Cs3 59.0(7) 2_655 .
O2 V2 Cs3 124.7(7) 5_656 .
Cs7 V2 Cs3 66.7(7) 7_565 .
Cs3 V2 Cs3 110(2) 6_556 .
V2 V2 Cs4 124.8(11) 5_556 .
O9 V2 Cs4 38.7(17) . .
O2 V2 Cs4 129.5(5) 1_455 .
O2 V2 Cs4 129.5(5) 6_456 .
O2 V2 Cs4 76.4(6) 2_655 .
O2 V2 Cs4 76.4(6) 5_656 .
Cs7 V2 Cs4 68.4(7) 7_565 .
Cs3 V2 Cs4 57.8(10) 6_556 .
Cs3 V2 Cs4 57.8(10) . .
V2 V2 Cs1 111.7(3) 5_556 1_556
O9 V2 Cs1 64.9(3) . 1_556
O2 V2 Cs1 151.4(6) 1_455 1_556
O2 V2 Cs1 64.4(4) 6_456 1_556
O2 V2 Cs1 127.7(5) 2_655 1_556
O2 V2 Cs1 55.0(4) 5_656 1_556
Cs7 V2 Cs1 72.3(2) 7_565 1_556
Cs3 V2 Cs1 8.6(11) 6_556 1_556
Cs3 V2 Cs1 118.6(10) . 1_556
Cs4 V2 Cs1 65.59(19) . 1_556
V2 V2 Cs1 111.7(3) 5_556 .
O9 V2 Cs1 64.9(3) . .
O2 V2 Cs1 64.4(4) 1_455 .
O2 V2 Cs1 151.4(6) 6_456 .
O2 V2 Cs1 55.0(4) 2_655 .
O2 V2 Cs1 127.7(5) 5_656 .
Cs7 V2 Cs1 72.3(2) 7_565 .
Cs3 V2 Cs1 118.6(10) 6_556 .
Cs3 V2 Cs1 8.6(11) . .
Cs4 V2 Cs1 65.59(19) . .
Cs1 V2 Cs1 127.3(3) 1_556 .
O7 Si1 O3 112.1(8) . .
O7 Si1 O3 112.1(8) . 6
O3 Si1 O3 106.7(9) . 6
O7 Si1 O1 109.5(8) . .
O3 Si1 O1 108.2(8) . .
O3 Si1 O1 108.2(8) 6 .
O7 Si1 Cs1 57.6(6) . 5_655
O3 Si1 Cs1 79.0(8) . 5_655
O3 Si1 Cs1 79.0(8) 6 5_655
O1 Si1 Cs1 167.1(6) . 5_655
O7 Si1 Cs3 54.2(8) . 5_655
O3 Si1 Cs3 89.4(13) . 5_655
O3 Si1 Cs3 73.4(9) 6 5_655
O1 Si1 Cs3 160.5(10) . 5_655
Cs1 Si1 Cs3 10.6(10) 5_655 5_655
O7 Si1 Cs3 54.2(8) . 2_655
O3 Si1 Cs3 73.4(9) . 2_655
O3 Si1 Cs3 89.4(13) 6 2_655
O1 Si1 Cs3 160.5(10) . 2_655
Cs1 Si1 Cs3 10.6(10) 5_655 2_655
Cs3 Si1 Cs3 19.7(16) 5_655 2_655
O7 Si1 Cs6 96.4(7) . 1_554
O3 Si1 Cs6 150.5(9) . 1_554
O3 Si1 Cs6 52.5(6) 6 1_554
O1 Si1 Cs6 67.2(4) . 1_554
Cs1 Si1 Cs6 111.9(5) 5_655 1_554
Cs3 Si1 Cs6 101.7(10) 5_655 1_554
Cs3 Si1 Cs6 121.1(9) 2_655 1_554
O7 Si1 Cs6 96.4(7) . .
O3 Si1 Cs6 52.5(6) . .
O3 Si1 Cs6 150.5(9) 6 .
O1 Si1 Cs6 67.2(4) . .
Cs1 Si1 Cs6 111.9(5) 5_655 .
Cs3 Si1 Cs6 121.1(9) 5_655 .
Cs3 Si1 Cs6 101.7(10) 2_655 .
Cs6 Si1 Cs6 134.3(8) 1_554 .
O7 Si1 Cs2 83.1(3) . 1_554
O3 Si1 Cs2 163.0(6) . 1_554
O3 Si1 Cs2 58.7(5) 6 1_554
O1 Si1 Cs2 71.86(16) . 1_554
Cs1 Si1 Cs2 104.50(12) 5_655 1_554
Cs3 Si1 Cs2 93.9(10) 5_655 1_554
Cs3 Si1 Cs2 112.5(6) 2_655 1_554
Cs6 Si1 Cs2 13.3(7) 1_554 1_554
Cs6 Si1 Cs2 136.3(4) . 1_554
O7 Si1 Cs2 83.1(3) . .
O3 Si1 Cs2 58.7(5) . .
O3 Si1 Cs2 163.0(6) 6 .
O1 Si1 Cs2 71.86(16) . .
Cs1 Si1 Cs2 104.50(12) 5_655 .
Cs3 Si1 Cs2 112.5(6) 5_655 .
Cs3 Si1 Cs2 93.9(10) 2_655 .
Cs6 Si1 Cs2 136.3(4) 1_554 .
Cs6 Si1 Cs2 13.3(7) . .
Cs2 Si1 Cs2 133.8(2) 1_554 .
O7 Si1 Cs7 107.2(6) . .
O3 Si1 Cs7 50.4(7) . .
O3 Si1 Cs7 140.2(8) 6 .
O1 Si1 Cs7 62.7(4) . .
Cs1 Si1 Cs7 118.7(4) 5_655 .
Cs3 Si1 Cs7 128.7(9) 5_655 .
Cs3 Si1 Cs7 109.0(9) 2_655 .
Cs6 Si1 Cs7 129.3(6) 1_554 .
Cs6 Si1 Cs7 11.0(6) . .
Cs2 Si1 Cs7 134.4(4) 1_554 .
Cs2 Si1 Cs7 24.2(5) . .
O6 Si2 O5 114.4(9) . .
O6 Si2 O5 114.4(9) . 6
O5 Si2 O5 104.3(11) . 6
O6 Si2 O1 109.4(8) . .
O5 Si2 O1 107.0(8) . .
O5 Si2 O1 107.0(8) 6 .
O6 Si2 Cs2 83.1(3) . 1_554
O5 Si2 Cs2 161.2(8) . 1_554
O5 Si2 Cs2 60.0(5) 6 1_554
O1 Si2 Cs2 71.24(19) . 1_554
O6 Si2 Cs2 83.1(3) . .
O5 Si2 Cs2 60.0(5) . .
O5 Si2 Cs2 161.2(8) 6 .
O1 Si2 Cs2 71.24(19) . .
Cs2 Si2 Cs2 132.63(15) 1_554 .
O6 Si2 Cs1 163.1(7) . 7_665
O5 Si2 Cs1 74.8(9) . 7_665
O5 Si2 Cs1 74.8(9) 6 7_665
O1 Si2 Cs1 53.7(5) . 7_665
Cs2 Si2 Cs1 90.2(2) 1_554 7_665
Cs2 Si2 Cs1 90.2(2) . 7_665
O6 Si2 Cs6 96.1(7) . .
O5 Si2 Cs6 55.1(6) . .
O5 Si2 Cs6 149.1(10) 6 .
O1 Si2 Cs6 64.9(4) . .
Cs2 Si2 Cs6 133.1(4) 1_554 .
Cs2 Si2 Cs6 13.1(7) . .
Cs1 Si2 Cs6 77.2(6) 7_665 .
O6 Si2 Cs6 96.1(7) . 1_554
O5 Si2 Cs6 149.1(10) . 1_554
O5 Si2 Cs6 55.1(6) 6 1_554
O1 Si2 Cs6 64.9(4) . 1_554
Cs2 Si2 Cs6 13.1(7) 1_554 1_554
Cs2 Si2 Cs6 133.1(4) . 1_554
Cs1 Si2 Cs6 77.2(6) 7_665 1_554
Cs6 Si2 Cs6 129.7(8) . 1_554
O6 Si2 Cs3 157.4(10) . 7_665
O5 Si2 Cs3 69.5(9) . 7_665
O5 Si2 Cs3 84.6(13) 6 7_665
O1 Si2 Cs3 50.6(7) . 7_665
Cs2 Si2 Cs3 97.3(5) 1_554 7_665
Cs2 Si2 Cs3 80.2(9) . 7_665
Cs1 Si2 Cs3 10.1(9) 7_665 7_665
Cs6 Si2 Cs3 67.2(11) . 7_665
Cs6 Si2 Cs3 84.6(8) 1_554 7_665
O6 Si2 Cs3 157.4(10) . 4
O5 Si2 Cs3 84.6(13) . 4
O5 Si2 Cs3 69.5(9) 6 4
O1 Si2 Cs3 50.6(7) . 4
Cs2 Si2 Cs3 80.2(9) 1_554 4
Cs2 Si2 Cs3 97.3(5) . 4
Cs1 Si2 Cs3 10.1(9) 7_665 4
Cs6 Si2 Cs3 84.6(8) . 4
Cs6 Si2 Cs3 67.2(11) 1_554 4
Cs3 Si2 Cs3 18.7(15) 7_665 4
O6 Si2 Cs7 107.1(6) . .
O5 Si2 Cs7 51.0(7) . .
O5 Si2 Cs7 138.2(10) 6 .
O1 Si2 Cs7 62.0(3) . .
Cs2 Si2 Cs7 132.9(4) 1_554 .
Cs2 Si2 Cs7 24.1(5) . .
Cs1 Si2 Cs7 66.7(5) 7_665 .
Cs6 Si2 Cs7 11.0(6) . .
Cs6 Si2 Cs7 126.5(6) 1_554 .
Cs3 Si2 Cs7 56.6(10) 7_665 .
Cs3 Si2 Cs7 74.5(7) 4 .
O2 Si3 O5 112.1(10) . 7_665
O2 Si3 O3 112.1(9) . .
O5 Si3 O3 106.3(9) 7_665 .
O2 Si3 O4 111.9(9) . .
O5 Si3 O4 108.0(11) 7_665 .
O3 Si3 O4 106.1(11) . .
O2 Si3 Cs7 134.9(7) . .
O5 Si3 Cs7 112.8(10) 7_665 .
O3 Si3 Cs7 58.7(7) . .
O4 Si3 Cs7 48.0(10) . .
O2 Si3 Cs7 83.3(7) . 7_665
O5 Si3 Cs7 59.9(6) 7_665 7_665
O3 Si3 Cs7 163.2(9) . 7_665
O4 Si3 Cs7 72.2(10) . 7_665
Cs7 Si3 Cs7 115.45(12) . 7_665
O2 Si3 Cs6 124.3(8) . .
O5 Si3 Cs6 123.6(11) 7_665 .
O3 Si3 Cs6 53.9(6) . .
O4 Si3 Cs6 52.4(10) . .
Cs7 Si3 Cs6 11.8(6) . .
Cs7 Si3 Cs6 123.5(4) 7_665 .
O2 Si3 Cs6 94.7(8) . 7_665
O5 Si3 Cs6 54.6(6) 7_665 7_665
O3 Si3 Cs6 152.3(10) . 7_665
O4 Si3 Cs6 67.8(10) . 7_665
Cs7 Si3 Cs6 107.0(5) . 7_665
Cs7 Si3 Cs6 11.4(6) 7_665 7_665
Cs6 Si3 Cs6 116.31(18) . 7_665
O2 Si3 Cs5 144.9(5) . 7_665
O5 Si3 Cs5 65.6(8) 7_665 7_665
O3 Si3 Cs5 101.4(8) . 7_665
O4 Si3 Cs5 45.9(8) . 7_665
Cs7 Si3 Cs5 57.1(6) . 7_665
Cs7 Si3 Cs5 65.0(6) 7_665 7_665
Cs6 Si3 Cs5 68.5(7) . 7_665
Cs6 Si3 Cs5 54.1(6) 7_665 7_665
O2 Si3 Cs3 44.0(5) . 2_655
O5 Si3 Cs3 122.7(12) 7_665 2_655
O3 Si3 Cs3 68.3(8) . 2_655
O4 Si3 Cs3 128.8(13) . 2_655
Cs7 Si3 Cs3 110.8(9) . 2_655
Cs7 Si3 Cs3 126.3(7) 7_665 2_655
Cs6 Si3 Cs3 99.5(10) . 2_655
Cs6 Si3 Cs3 137.5(8) 7_665 2_655
Cs5 Si3 Cs3 167.7(7) 7_665 2_655
O2 Si3 Cs2 113.4(5) . .
O5 Si3 Cs2 134.1(9) 7_665 .
O3 Si3 Cs2 49.9(5) . .
O4 Si3 Cs2 59.1(10) . .
Cs7 Si3 Cs2 23.8(6) . .
Cs7 Si3 Cs2 131.3(3) 7_665 .
Cs6 Si3 Cs2 12.1(7) . .
Cs6 Si3 Cs2 125.8(4) 7_665 .
Cs5 Si3 Cs2 80.4(2) 7_665 .
Cs3 Si3 Cs2 87.7(8) 2_655 .
O2 Si3 Cs1 46.4(5) . 5_655
O5 Si3 Cs1 113.1(7) 7_665 5_655
O3 Si3 Cs1 67.7(8) . 5_655
O4 Si3 Cs1 138.5(9) . 5_655
Cs7 Si3 Cs1 116.3(5) . 5_655
Cs7 Si3 Cs1 125.0(6) 7_665 5_655
Cs6 Si3 Cs1 105.6(6) . 5_655
Cs6 Si3 Cs1 135.3(6) 7_665 5_655
Cs5 Si3 Cs1 168.6(2) 7_665 5_655
Cs3 Si3 Cs1 9.7(10) 2_655 5_655
Cs2 Si3 Cs1 94.2(2) . 5_655
Si1 O1 Si2 133.3(9) . .
Si1 O1 Cs1 124.5(7) . 7_665
Si2 O1 Cs1 102.3(7) . 7_665
Si1 O1 Cs3 119.1(11) . 7_665
Si2 O1 Cs3 106.6(9) . 7_665
Cs1 O1 Cs3 12.5(12) 7_665 7_665
Si1 O1 Cs3 119.1(11) . 4
Si2 O1 Cs3 106.6(9) . 4
Cs1 O1 Cs3 12.5(12) 7_665 4
Cs3 O1 Cs3 23.2(19) 7_665 4
Si1 O1 Cs6 88.0(5) . 1_554
Si2 O1 Cs6 90.5(5) . 1_554
Cs1 O1 Cs6 92.1(8) 7_665 1_554
Cs3 O1 Cs6 103.7(12) 7_665 1_554
Cs3 O1 Cs6 80.4(12) 4 1_554
Si1 O1 Cs6 88.0(5) . .
Si2 O1 Cs6 90.5(5) . .
Cs1 O1 Cs6 92.1(8) 7_665 .
Cs3 O1 Cs6 80.4(12) 7_665 .
Cs3 O1 Cs6 103.7(12) 4 .
Cs6 O1 Cs6 175.3(13) 1_554 .
Si1 O1 Cs7 93.8(5) . .
Si2 O1 Cs7 94.5(5) . .
Cs1 O1 Cs7 79.7(6) 7_665 .
Cs3 O1 Cs7 68.0(11) 7_665 .
Cs3 O1 Cs7 91.2(11) 4 .
Cs6 O1 Cs7 171.2(12) 1_554 .
Cs6 O1 Cs7 12.5(6) . .
Si1 O1 Cs7 93.8(5) . 1_554
Si2 O1 Cs7 94.5(5) . 1_554
Cs1 O1 Cs7 79.7(6) 7_665 1_554
Cs3 O1 Cs7 91.2(11) 7_665 1_554
Cs3 O1 Cs7 68.0(11) 4 1_554
Cs6 O1 Cs7 12.5(6) 1_554 1_554
Cs6 O1 Cs7 171.2(12) . 1_554
Cs7 O1 Cs7 158.9(12) . 1_554
Si1 O1 Cs2 83.5(3) . 1_554
Si2 O1 Cs2 84.0(3) . 1_554
Cs1 O1 Cs2 105.6(3) 7_665 1_554
Cs3 O1 Cs2 117.4(10) 7_665 1_554
Cs3 O1 Cs2 94.2(10) 4 1_554
Cs6 O1 Cs2 14.0(7) 1_554 1_554
Cs6 O1 Cs2 162.1(9) . 1_554
Cs7 O1 Cs2 174.6(7) . 1_554
Cs7 O1 Cs2 26.4(6) 1_554 1_554
Si1 O1 Cs2 83.5(3) . .
Si2 O1 Cs2 84.0(3) . .
Cs1 O1 Cs2 105.6(3) 7_665 .
Cs3 O1 Cs2 94.2(10) 7_665 .
Cs3 O1 Cs2 117.4(10) 4 .
Cs6 O1 Cs2 162.1(9) 1_554 .
Cs6 O1 Cs2 14.0(7) . .
Cs7 O1 Cs2 26.4(6) . .
Cs7 O1 Cs2 174.6(7) 1_554 .
Cs2 O1 Cs2 148.3(6) 1_554 .
Si3 O2 V2 123.8(8) . 1_655
Si3 O2 V2 140.8(7) . 5_656
V2 O2 V2 36.0(5) 1_655 5_656
Si3 O2 Cs3 114.6(7) . 2_655
V2 O2 Cs3 117.5(8) 1_655 2_655
V2 O2 Cs3 84.2(9) 5_656 2_655
Si3 O2 Cs1 112.6(6) . 5_655
V2 O2 Cs1 122.8(7) 1_655 5_655
V2 O2 Cs1 92.6(5) 5_656 5_655
Cs3 O2 Cs1 12.4(13) 2_655 5_655
Si3 O2 Cs3 109.1(7) . 1_655
V2 O2 Cs3 76.4(11) 1_655 1_655
V2 O2 Cs3 97.6(8) 5_656 1_655
Cs3 O2 Cs3 105(2) 2_655 1_655
Cs1 O2 Cs3 94.8(9) 5_655 1_655
Si3 O2 Cs1 107.5(6) . 1_655
V2 O2 Cs1 86.7(5) 1_655 1_655
V2 O2 Cs1 104.1(5) 5_656 1_655
Cs3 O2 Cs1 96.0(12) 2_655 1_655
Cs1 O2 Cs1 85.2(4) 5_655 1_655
Cs3 O2 Cs1 11.4(12) 1_655 1_655
Si3 O2 Cs3 108.0(7) . 5_655
V2 O2 Cs3 127.8(8) 1_655 5_655
V2 O2 Cs3 98.4(6) 5_656 5_655
Cs3 O2 Cs3 17.2(14) 2_655 5_655
Cs1 O2 Cs3 5.8(4) 5_655 5_655
Cs3 O2 Cs3 93.2(12) 1_655 5_655
Cs1 O2 Cs3 83.1(3) 1_655 5_655
Si1 O3 Si3 154.6(9) . .
Si1 O3 Cs6 103.9(7) . .
Si3 O3 Cs6 101.3(8) . .
Si1 O3 Cs7 107.7(8) . .
Si3 O3 Cs7 96.2(8) . .
Cs6 O3 Cs7 13.8(7) . .
Si1 O3 Cs2 97.2(5) . .
Si3 O3 Cs2 108.0(6) . .
Cs6 O3 Cs2 15.5(8) . .
Cs7 O3 Cs2 29.3(6) . .
Si1 O3 Cs3 82.3(9) . 2_655
Si3 O3 Cs3 87.7(8) . 2_655
Cs6 O3 Cs3 120.5(14) . 2_655
Cs7 O3 Cs3 133.6(13) . 2_655
Cs2 O3 Cs3 106.1(11) . 2_655
Si1 O3 Cs4 101.8(8) . 5_656
Si3 O3 Cs4 92.0(8) . 5_656
Cs6 O3 Cs4 64.0(8) . 5_656
Cs7 O3 Cs4 76.7(7) . 5_656
Cs2 O3 Cs4 50.9(3) . 5_656
Cs3 O3 Cs4 57.0(11) 2_655 5_656
Si1 O3 Cs1 76.9(8) . 5_655
Si3 O3 Cs1 89.1(8) . 5_655
Cs6 O3 Cs1 130.4(10) . 5_655
Cs7 O3 Cs1 143.8(8) . 5_655
Cs2 O3 Cs1 115.5(6) . 5_655
Cs3 O3 Cs1 10.6(10) 2_655 5_655
Cs4 O3 Cs1 67.4(4) 5_656 5_655
Si3 O4 Si3 129.8(15) 6_556 .
Si3 O4 Cs7 107.7(10) 6_556 .
Si3 O4 Cs7 107.7(10) . .
Si3 O4 Cs5 111.1(9) 6_556 7_665
Si3 O4 Cs5 111.1(9) . 7_665
Cs7 O4 Cs5 76.2(9) . 7_665
Si3 O4 Cs6 102.6(11) 6_556 .
Si3 O4 Cs6 102.6(11) . .
Cs7 O4 Cs6 14.6(7) . .
Cs5 O4 Cs6 90.8(10) 7_665 .
Si3 O4 Cs2 97.5(10) 6_556 .
Si3 O4 Cs2 97.5(10) . .
Cs7 O4 Cs2 27.7(7) . .
Cs5 O4 Cs2 103.8(7) 7_665 .
Cs6 O4 Cs2 13.0(8) . .
Si3 O4 Cs6 87.5(11) 6_556 7_665
Si3 O4 Cs6 87.5(11) . 7_665
Cs7 O4 Cs6 140.2(10) . 7_665
Cs5 O4 Cs6 64.0(9) 7_665 7_665
Cs6 O4 Cs6 154.8(8) . 7_665
Cs2 O4 Cs6 167.9(10) . 7_665
Si3 O4 Cs7 82.4(10) 6_556 7_665
Si3 O4 Cs7 82.4(10) . 7_665
Cs7 O4 Cs7 152.5(8) . 7_665
Cs5 O4 Cs7 76.3(9) 7_665 7_665
Cs6 O4 Cs7 167.1(11) . 7_665
Cs2 O4 Cs7 179.9(9) . 7_665
Cs6 O4 Cs7 12.3(6) 7_665 7_665
Si3 O4 Cs2 93.4(10) 6_556 7_665
Si3 O4 Cs2 93.4(10) . 7_665
Cs7 O4 Cs2 126.3(10) . 7_665
Cs5 O4 Cs2 50.2(5) 7_665 7_665
Cs6 O4 Cs2 140.9(11) . 7_665
Cs2 O4 Cs2 154.0(7) . 7_665
Cs6 O4 Cs2 13.9(7) 7_665 7_665
Cs7 O4 Cs2 26.1(6) 7_665 7_665
Si2 O5 Si3 156.6(10) . 7_565
Si2 O5 Cs6 101.5(7) . .
Si3 O5 Cs6 101.8(7) 7_565 .
Si2 O5 Cs7 107.1(8) . .
Si3 O5 Cs7 95.1(7) 7_565 .
Cs6 O5 Cs7 13.6(7) . .
Si2 O5 Cs2 95.9(6) . .
Si3 O5 Cs2 107.2(6) 7_565 .
Cs6 O5 Cs2 15.3(8) . .
Cs7 O5 Cs2 28.9(6) . .
Si2 O5 Cs5 102.4(9) . .
Si3 O5 Cs5 90.3(9) 7_565 .
Cs6 O5 Cs5 62.7(8) . .
Cs7 O5 Cs5 74.1(6) . .
Cs2 O5 Cs5 49.5(3) . .
Si2 O5 Cs3 87.3(10) . 7_665
Si3 O5 Cs3 95.8(9) 7_565 7_665
Cs6 O5 Cs3 76.7(13) . 7_665
Cs7 O5 Cs3 65.3(12) . 7_665
Cs2 O5 Cs3 90.6(11) . 7_665
Cs5 O5 Cs3 139.3(11) . 7_665
Si2 O5 Cs1 81.6(9) . 7_665
Si3 O5 Cs1 97.5(9) 7_565 7_665
Cs6 O5 Cs1 86.7(8) . 7_665
Cs7 O5 Cs1 75.7(7) . 7_665
Cs2 O5 Cs1 100.0(5) . 7_665
Cs5 O5 Cs1 149.4(5) . 7_665
Cs3 O5 Cs1 10.7(10) 7_665 7_665
Si2 O6 V1 138.1(10) . .
Si2 O6 Cs3 116.1(8) . 6
V1 O6 Cs3 105.1(6) . 6
Si2 O6 Cs3 116.1(8) . .
V1 O6 Cs3 105.1(6) . .
Cs3 O6 Cs3 21(2) 6 .
Si2 O6 Cs5 98.7(4) . 1_554
V1 O6 Cs5 93.3(4) . 1_554
Cs3 O6 Cs5 62.2(10) 6 1_554
Cs3 O6 Cs5 83.5(10) . 1_554
Si2 O6 Cs5 98.7(4) . .
V1 O6 Cs5 93.3(4) . .
Cs3 O6 Cs5 83.5(10) 6 .
Cs3 O6 Cs5 62.2(10) . .
Cs5 O6 Cs5 145.7(6) 1_554 .
Si2 O6 Cs1 117.7(8) . .
V1 O6 Cs1 104.2(6) . .
Cs3 O6 Cs1 10.7(10) 6 .
Cs3 O6 Cs1 10.7(10) . .
Cs5 O6 Cs1 72.9(3) 1_554 .
Cs5 O6 Cs1 72.9(3) . .
Si1 O7 V1 137.7(10) . .
Si1 O7 Cs3 102.6(10) . 2_655
V1 O7 Cs3 118.8(10) . 2_655
Si1 O7 Cs3 102.6(10) . 5_655
V1 O7 Cs3 118.8(10) . 5_655
Cs3 O7 Cs3 24(2) 2_655 5_655
Si1 O7 Cs1 98.6(7) . 5_655
V1 O7 Cs1 123.7(6) . 5_655
Cs3 O7 Cs1 12.6(12) 2_655 5_655
Cs3 O7 Cs1 12.6(12) 5_655 5_655
Si1 O7 Cs4 103.7(6) . 5_655
V1 O7 Cs4 89.5(6) . 5_655
Cs3 O7 Cs4 84.5(10) 2_655 5_655
Cs3 O7 Cs4 61.2(12) 5_655 5_655
Cs1 O7 Cs4 73.7(4) 5_655 5_655
Si1 O7 Cs4 103.7(6) . 5_656
V1 O7 Cs4 89.5(6) . 5_656
Cs3 O7 Cs4 61.2(12) 2_655 5_656
Cs3 O7 Cs4 84.5(10) 5_655 5_656
Cs1 O7 Cs4 73.7(4) 5_655 5_656
Cs4 O7 Cs4 139.8(8) 5_655 5_656
V1 O8 Cs4 128.7(6) . 5_656
V1 O8 Cs4 128.7(6) . .
Cs4 O8 Cs4 102.6(12) 5_656 .
V1 O8 Cs5 127.6(5) . .
Cs4 O8 Cs5 99.9(9) 5_656 .
Cs4 O8 Cs5 20.9(7) . .
V1 O8 Cs5 127.6(5) . 5_656
Cs4 O8 Cs5 20.9(7) 5_656 5_656
Cs4 O8 Cs5 99.9(9) . 5_656
Cs5 O8 Cs5 104.8(11) . 5_656
V1 O8 Cs2 126.2(5) . .
Cs4 O8 Cs2 61.4(7) 5_656 .
Cs4 O8 Cs2 74.9(9) . .
Cs5 O8 Cs2 57.0(5) . .
Cs5 O8 Cs2 79.8(7) 5_656 .
V1 O8 Cs2 126.2(5) . 5_656
Cs4 O8 Cs2 74.9(9) 5_656 5_656
Cs4 O8 Cs2 61.4(7) . 5_656
Cs5 O8 Cs2 79.8(7) . 5_656
Cs5 O8 Cs2 57.0(5) 5_656 5_656
Cs2 O8 Cs2 107.6(10) . 5_656
V1 O8 Cs6 118.4(5) . .
Cs4 O8 Cs6 64.7(8) 5_656 .
Cs4 O8 Cs6 80.4(9) . .
Cs5 O8 Cs6 61.4(6) . .
Cs5 O8 Cs6 84.2(7) 5_656 .
Cs2 O8 Cs6 7.9(3) . .
Cs2 O8 Cs6 115.4(10) 5_656 .
V1 O8 Cs6 118.4(5) . 5_656
Cs4 O8 Cs6 80.4(9) 5_656 5_656
Cs4 O8 Cs6 64.7(8) . 5_656
Cs5 O8 Cs6 84.2(7) . 5_656
Cs5 O8 Cs6 61.4(6) 5_656 5_656
Cs2 O8 Cs6 115.4(10) . 5_656
Cs2 O8 Cs6 7.9(3) 5_656 5_656
Cs6 O8 Cs6 123.2(11) . 5_656
OW1 O9 V2 139(4) 7_565 .
OW1 O9 Cs7 12(2) 7_565 7_565
V2 O9 Cs7 127(3) . 7_565
OW1 O9 Cs4 103(3) 7_565 .
V2 O9 Cs4 118(2) . .
Cs7 O9 Cs4 115(2) 7_565 .
OW1 O9 Cs6 17(3) 7_565 7_565
V2 O9 Cs6 122(3) . 7_565
Cs7 O9 Cs6 4.3(10) 7_565 7_565
Cs4 O9 Cs6 119.7(17) . 7_565
OW1 O9 Cs5 81(3) 7_565 .
V2 O9 Cs5 140(2) . .
Cs7 O9 Cs5 93.5(17) 7_565 .
Cs4 O9 Cs5 21.9(9) . .
Cs6 O9 Cs5 97.8(13) 7_565 .
OW1 O9 Cs3 94.4(10) 7_565 6_556
V2 O9 Cs3 94.0(11) . 6_556
Cs7 O9 Cs3 96.7(8) 7_565 6_556
Cs4 O9 Cs3 78.0(13) . 6_556
Cs6 O9 Cs3 97.5(8) 7_565 6_556
Cs5 O9 Cs3 79.5(14) . 6_556
OW1 O9 Cs3 94.4(10) 7_565 .
V2 O9 Cs3 94.0(11) . .
Cs7 O9 Cs3 96.7(8) 7_565 .
Cs4 O9 Cs3 78.0(13) . .
Cs6 O9 Cs3 97.5(8) 7_565 .
Cs5 O9 Cs3 79.5(14) . .
Cs3 O9 Cs3 156(2) 6_556 .
OW1 O9 Cs1 96.0(6) 7_565 .
V2 O9 Cs1 89.2(6) . .
Cs7 O9 Cs1 97.1(6) 7_565 .
Cs4 O9 Cs1 83.0(9) . .
Cs6 O9 Cs1 97.5(6) 7_565 .
Cs5 O9 Cs1 85.2(9) . .
Cs3 O9 Cs1 160.0(19) 6_556 .
Cs3 O9 Cs1 5.8(11) . .
OW1 O9 Cs1 96.0(6) 7_565 1_556
V2 O9 Cs1 89.2(6) . 1_556
Cs7 O9 Cs1 97.1(6) 7_565 1_556
Cs4 O9 Cs1 83.0(9) . 1_556
Cs6 O9 Cs1 97.5(6) 7_565 1_556
Cs5 O9 Cs1 85.2(9) . 1_556
Cs3 O9 Cs1 5.8(11) 6_556 1_556
Cs3 O9 Cs1 160.0(19) . 1_556
Cs1 O9 Cs1 163.3(15) . 1_556
OW1 O9 Cs2 22(3) 7_565 7_565
V2 O9 Cs2 118(2) . 7_565
Cs7 O9 Cs2 9.1(10) 7_565 7_565
Cs4 O9 Cs2 124.5(15) . 7_565
Cs6 O9 Cs2 4.8(6) 7_565 7_565
Cs5 O9 Cs2 102.6(11) . 7_565
Cs3 O9 Cs2 98.2(8) 6_556 7_565
Cs3 O9 Cs2 98.2(8) . 7_565
Cs1 O9 Cs2 97.7(6) . 7_565
Cs1 O9 Cs2 97.7(6) 1_556 7_565
Cs7 OW1 O9 141(7) . 7_665
Cs7 OW1 Cs6 5(3) . .
O9 OW1 Cs6 147(5) 7_665 .
Cs7 OW1 Cs2 4(4) . .
O9 OW1 Cs2 145(4) 7_665 .
Cs6 OW1 Cs2 1.4(12) . .
Cs7 OW1 Cs5 149(6) . 7_665
O9 OW1 Cs5 70(3) 7_665 7_665
Cs6 OW1 Cs5 144(3) . 7_665
Cs2 OW1 Cs5 145(2) . 7_665
Cs7 OW1 Cs4 167(6) . 7_665
O9 OW1 Cs4 51(3) 7_665 7_665
Cs6 OW1 Cs4 162(3) . 7_665
Cs2 OW1 Cs4 163(2) . 7_665
Cs5 OW1 Cs4 18.4(7) 7_665 7_665
Cs7 OW1 Cs3 120.1(17) . 4_556
O9 OW1 Cs3 59.6(11) 7_665 4_556
Cs6 OW1 Cs3 121.1(12) . 4_556
Cs2 OW1 Cs3 120.8(12) . 4_556
Cs5 OW1 Cs3 70.5(14) 7_665 4_556
Cs4 OW1 Cs3 63.4(13) 7_665 4_556
Cs7 OW1 Cs3 120.1(17) . 7_665
O9 OW1 Cs3 59.6(11) 7_665 7_665
Cs6 OW1 Cs3 121.1(12) . 7_665
Cs2 OW1 Cs3 120.8(12) . 7_665
Cs5 OW1 Cs3 70.5(14) 7_665 7_665
Cs4 OW1 Cs3 63.4(13) 7_665 7_665
Cs3 OW1 Cs3 115(2) 4_556 7_665
Cs5 OW2 Cs4 108(8) . .
Cs5 OW2 Cs2 81(6) . .
Cs4 OW2 Cs2 172(8) . .
Cs5 OW2 Cs2 173(6) . 5_656
Cs4 OW2 Cs2 66(6) . 5_656
Cs2 OW2 Cs2 105.9(19) . 5_656
Cs5 OW2 Cs6 73(5) . .
Cs4 OW2 Cs6 180(7) . .
Cs2 OW2 Cs6 8.1(6) . .
Cs2 OW2 Cs6 114.0(17) 5_656 .
Cs2 OW3 Cs6 14(4) . .
Cs2 OW3 Cs7 21(4) . .
Cs6 OW3 Cs7 6.4(14) . .
Cs2 OW3 Cs5 151(7) . .
Cs6 OW3 Cs5 136(3) . .
Cs7 OW3 Cs5 130(3) . .
Cs2 OW3 Cs4 94(7) . 5_656
Cs6 OW3 Cs4 108(4) . 5_656
Cs7 OW3 Cs4 115(3) . 5_656
Cs5 OW3 Cs4 116(2) . 5_656
Cs2 OW3 Cs4 168(7) . .
Cs6 OW3 Cs4 154(4) . .
Cs7 OW3 Cs4 147(3) . .
Cs5 OW3 Cs4 17.4(9) . .
Cs4 OW3 Cs4 98.1(17) 5_656 .
Cs2 OW3 Cs5 108(7) . 5_656
Cs6 OW3 Cs5 122(4) . 5_656
Cs7 OW3 Cs5 129(3) . 5_656
Cs5 OW3 Cs5 101.3(19) . 5_656
Cs4 OW3 Cs5 14.2(8) 5_656 5_656
Cs4 OW3 Cs5 83.9(13) . 5_656
Cs1 OW4 Cs3 23(3) . .
Cs1 OW4 Cs3 23(3) . 6
Cs3 OW4 Cs3 43(5) . 6
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cs1 Cs3 0.70(7) .
Cs1 Cs3 0.70(7) 6
Cs1 OW4 1.42(16) .
Cs1 O1 3.180(16) 7_565
Cs1 O7 3.194(18) 5_655
Cs1 O2 3.196(14) 5_655
Cs1 O2 3.196(14) 2_655
Cs1 O2 3.519(15) 6_455
Cs1 O2 3.519(15) 1_455
Cs1 O9 3.529(7) .
Cs1 O9 3.529(7) 1_554
Cs1 O6 3.676(18) .
Cs2 OW3 0.60(6) .
Cs2 Cs6 0.88(4) .
Cs2 Cs7 1.64(4) .
Cs2 OW1 2.36(7) .
Cs2 Cs5 2.878(15) .
Cs2 OW2 2.91(6) .
Cs2 Cs4 3.04(2) 5_656
Cs2 O8 3.06(2) .
Cs2 O8 3.06(2) 5_656
Cs2 O3 3.268(14) 6_556
Cs2 O3 3.268(14) .
Cs2 OW2 3.27(8) 5_656
Cs3 Cs3 1.29(11) 6
Cs3 OW4 1.74(15) .
Cs3 O9 2.91(5) .
Cs3 O2 2.995(19) 2_655
Cs3 O7 3.13(2) 5_655
Cs3 O1 3.20(2) 7_565
Cs3 OW1 3.37(6) 7_565
Cs3 O2 3.40(2) 1_455
Cs3 V2 3.48(2) .
Cs3 O6 3.48(4) .
Cs3 Cs4 3.53(6) .
Cs4 OW2 0.72(4) .
Cs4 Cs5 1.07(3) .
Cs4 O9 2.68(6) .
Cs4 O8 2.89(3) 5_656
Cs4 O8 2.89(3) .
Cs4 OW3 2.95(6) 5_656
Cs4 OW3 3.03(8) .
Cs4 Cs2 3.04(2) 5_656
Cs4 OW1 3.34(7) 7_565
Cs4 Cs3 3.53(6) 6_556
Cs5 OW2 0.60(6) .
Cs5 OW3 2.34(8) .
Cs5 O9 2.86(5) .
Cs5 O8 2.96(2) 5_656
Cs5 O8 2.96(2) .
Cs5 O4 2.99(3) 7_565
Cs5 OW1 3.01(7) 7_565
Cs5 Cs6 3.53(4) .
Cs5 O5 3.54(3) 6_556
Cs5 O5 3.54(3) .
Cs6 Cs7 0.77(4) .
Cs6 OW3 1.45(8) .
Cs6 OW1 1.49(7) .
Cs6 O9 2.85(6) 7_665
Cs6 O4 3.05(4) .
Cs6 O3 3.10(2) 6_556
Cs6 O3 3.10(2) .
Cs6 O5 3.23(2) .
Cs6 O5 3.23(2) 6_556
Cs6 O1 3.4947(18) 1_556
Cs6 O1 3.4947(18) .
Cs7 OW1 0.72(6) .
Cs7 O9 2.10(5) 7_665
Cs7 OW3 2.19(7) .
Cs7 O4 2.93(4) .
Cs7 O3 3.22(2) 6_556
Cs7 O3 3.22(2) .
Cs7 O5 3.26(2) .
Cs7 O5 3.26(2) 6_556
Cs7 V2 3.40(3) 7_665
Cs7 O1 3.552(7) .
V1 O8 1.68(3) .
V1 O8 1.68(3) 5_655
V1 O6 1.889(15) 5_655
V1 O6 1.889(15) .
V1 O7 1.894(15) 5_655
V1 O7 1.894(15) .
V1 Cs4 4.158(13) 1_554
V1 Cs4 4.158(13) 5_656
V1 Cs4 4.158(13) 5_655
V1 Cs5 4.208(10) 1_554
V2 V2 1.245(16) 5_556
V2 O9 1.70(4) .
V2 O2 1.891(13) 1_455
V2 O2 1.891(13) 6_456
V2 O2 2.090(14) 2_655
V2 O2 2.090(14) 5_656
V2 Cs7 3.40(3) 7_565
V2 Cs3 3.48(2) 6_556
V2 Cs1 3.897(6) 1_556
Si1 O7 1.523(15) .
Si1 O3 1.563(13) .
Si1 O3 1.563(13) 6
Si1 O1 1.591(15) .
Si1 Cs1 3.739(9) 5_655
Si1 Cs3 3.771(15) 5_655
Si1 Cs3 3.771(15) 2_655
Si1 Cs6 3.788(11) 1_554
Si1 Cs2 3.796(3) 1_554
Si2 O6 1.515(15) .
Si2 O5 1.563(13) .
Si2 O5 1.563(13) 6
Si2 O1 1.604(14) .
Si2 Cs2 3.813(2) 1_554
Si2 Cs1 3.854(9) 7_665
Si2 Cs6 3.858(12) 1_554
Si2 Cs3 3.97(3) 7_665
Si2 Cs3 3.97(3) 4
Si3 O2 1.579(14) .
Si3 O5 1.587(14) 7_665
Si3 O3 1.602(13) .
Si3 O4 1.624(11) .
Si3 Cs7 3.75(2) 7_665
Si3 Cs6 3.88(2) 7_665
Si3 Cs5 3.88(2) 7_665
Si3 Cs3 3.924(15) 2_655
Si3 Cs1 4.072(8) 5_655
O1 Cs1 3.180(16) 7_665
O1 Cs3 3.20(2) 7_665
O1 Cs3 3.20(2) 4
O1 Cs6 3.4947(18) 1_554
O1 Cs7 3.552(7) 1_554
O1 Cs2 3.630(5) 1_554
O2 V2 1.891(13) 1_655
O2 V2 2.090(14) 5_656
O2 Cs3 2.995(19) 2_655
O2 Cs1 3.196(14) 5_655
O2 Cs3 3.40(2) 1_655
O2 Cs1 3.519(15) 1_655
O2 Cs3 3.80(6) 5_655
O3 Cs3 3.65(3) 2_655
O3 Cs4 3.74(3) 5_656
O3 Cs1 3.77(2) 5_655
O4 Si3 1.624(11) 6_556
O4 Cs5 2.99(3) 7_665
O4 Cs6 3.60(4) 7_665
O4 Cs7 3.61(4) 7_665
O4 Cs2 3.65(3) 7_665
O5 Si3 1.587(14) 7_565
O5 Cs3 3.72(3) 7_665
O5 Cs1 3.76(2) 7_665
O6 Cs3 3.48(4) 6
O6 Cs5 3.654(6) 1_554
O7 Cs3 3.13(2) 2_655
O7 Cs3 3.13(2) 5_655
O7 Cs1 3.194(18) 5_655
O7 Cs4 3.718(9) 5_655
O7 Cs4 3.718(9) 5_656
O8 Cs4 2.89(3) 5_656
O8 Cs5 2.96(2) 5_656
O8 Cs2 3.06(2) 5_656
O8 Cs6 3.80(4) 5_656
O9 OW1 1.48(7) 7_565
O9 Cs7 2.10(5) 7_565
O9 Cs6 2.85(6) 7_565
O9 Cs3 2.91(5) 6_556
O9 Cs1 3.529(7) 1_556
O9 Cs2 3.68(4) 7_565
OW1 O9 1.48(7) 7_665
OW1 Cs5 3.01(7) 7_665
OW1 Cs4 3.34(7) 7_665
OW1 Cs3 3.37(6) 4_556
OW1 Cs3 3.37(6) 7_665
OW2 Cs2 3.27(8) 5_656
OW3 Cs4 2.95(6) 5_656
OW3 Cs5 3.64(6) 5_656
OW4 Cs3 1.74(15) 6
